1 TRANSPORT PROBLEMS 2007 PROBLEMY TRANSPORTU Tom 2 Zeszyt 3 Maciej BOLDYS*, Marcin STAŃCZYK Silesian University of Technology, Faculty of Transport Krasińskiego St. 8, Katowice, Poland *Corresponding author. THE INFLUENCE OF THE STEEL CHEMICAL COMPOSITION ONTO THE POSSIBILITIES OF USING IT IN THE PROCESS OF COLD SHAPING Summary. In the paper it was shown what influence the steel chemical composition has onto the possibilities of using it in the process of cold shaping. Researches were made on closed sections used in constructions of automotive vehicles, made of steel quality S235JRH, S355J2H and L360MB. They included the analysis of the chemical composition, the examination of their mechanical properties and the hardness measurement. Moreover, for steel S235JRH and S355J2H the examination of microstructure was made. WPŁYW SKŁADU CHEMICZNEGO STALI NA MOśLIWOŚCI WYKORZYSTANIA JEJ W PROCESIE KSZTAŁTOWANIA NA ZIMNO Streszczenie. W opracowaniu przedstawiono wpływ składu chemicznego stali na moŝliwość kształtowania jej metodami przeróbki plastycznej na zimno. Badania przeprowadzono na profilach zamkniętych wykorzystywanych w budowie pojazdów samochodowych, wykonanych ze stali S235JRH, S355J2H oraz L360MB. Obejmowały one analizę składu chemicznego stali, badania ich właściwości mechanicznych oraz pomiary twardości. Ponadto, dla stali S235JRH oraz S355J2H wykonano badania mikrostruktury. 1. INTRODUCTION Contemporary vehicles are characterized by complicated structure, first of all in the ground of gradable durability of their construction . Although the technology is constantly developing and new construction materials are used (composite, plastic, high-strength steel) the contribution of construction materials is still the highest which amounts to about 68% (Fig. 1.) . The basic technology of producing vehicles parts is the cold malleable processing. The closed weldable shapes or half-closed produced in the process of cold forming from steel band have found wide usage in vehicle production. As a batch material, they use steel with alloy addition which have the influence on the mechanical proprieties and the corrosive resistance of a construction. The introduction of alloy addition causes the decrease of the steel ductility, which influences the possibilities of using it in the process of cold forming.
2 82 M. Boldys, M. Stańczyk Fig. 1. The contribution of construction materials used in vehicles production  Rys. 1. Udział stali konstrukcyjnych stosowanych w budowie pojazdów  2. CHARACTERISTIC AND PROPERTIES OF A MATERIAL Cold plastic processing causes the strengthening of sheet steel, improving the durability properties of a part . The closed weldable shapes or half-closed are made of steel : non alloy; low-alloyed fine-grained; low-alloyed thermal-plastic treatment; low-alloyed quenching and tempering. Sheet steel is the batch material used in the production of closed weldable shapes. It should be characterized as having high resistance properties (R m and R e ). Moreover, because of the wide range of the exploitation temperature in the contemporary vehicles (e.g. minus 20 0 C) construction materials should have high resistance against brittle splitting. These proprieties are achieved by proper selection of the chemical composition, proper technology of melting and the use of malleable and thermal processing. One of the most importing properties of steel used in the production of closed weldable shapes is its weldability. The proper weldability enables gaining needed propriety of the shape after welding. Three factors are decisive: metallurgical; technological; structural. In case of bonded shapes it is unacceptable that in the zone of heat influence (HAZ) there is a hardening structure with high hardness and low ductility. Those structures can cause the material cracking as a result of natural tension or exploitation activities. In order to reduce the risk of arising hardening structure the chemical composition of a material is modified on the grounds of coal equivalent: C E = C + Mn/6 + (Cr + Mo + V)/5 + (Ni + Cu)/15, [%] (1)
3 The influence of the steel chemical 83 Steel is thought to be well for welding in case when C E 0,45%. In other cases steel requires additional operations like prior heating before welding, controlled cooling or the thermal processing . The technology of manufacturing has a big influence on the proprieties of the steel band used in shapes. In order to have the fine-grained structure of steel the procedure of blowing the metal bathing by nitrogen or calcium cyanamide is used. Regulated steel rolling, which is done in two ranges of temperature, affects the creation of fine-grained ferritic structure. The prior rolling is done in relatively high temperature, however the final rolling is done in low temperature in small deformability and numerous culverts with fast cooling . The elementary group of steel used in the welding shapes is the non alloy construction steel. The steel belongs to quality steel. The chemical composition and the mechanical proprieties of steel are given in the norms PN-EN :205 (U)  and PN-EN :205 (U) . Chosen types of steel and the required chemical composition are shown in the table 1, and in the table 2 their mechanical proprieties. Table 1 The chemical composition of examined types of non alloy construction steel [7,12] Steel type Maximal element concentration [%] C E C Si Mn P S N S235JR 0,35 0,17-1,40 0,035 0,035 0,012 S355JR 0,45 0,24 0,55 1,60 0,035 0,035 0,012 L360MB 0,41 0,16 0,45 1,60 0,025 0,020 - C E coal equivalent Steel type The mechanical proprieties of examined types of non alloy construction steel [7,12] R eh [MPa] min. Mechanical proprieties R m [MPa] A [%] min. Table 2 KV [J] (for 20 o C) min. S235JR S355JR L360MB Results of examination The examinations of chosen steel were to define its usefulness in the process of cold shaping on the basis of the chemical composition analysis, the mechanical proprieties and the hardness distribution in the zone welded by induction and in the bending site. The shapes which were used in the examination: a) 100x150x6,3 S235JRH steel (thermal-plastic treatment batch), b) 100x100x4 S355J2H steel (thermal-plastic treatment batch), c) Ø 273x6,35 L360MB steel. Chosen examination results were averaged and presented in a graphical form and in a table Chemical composition analysis The chemical composition analysis was made by the spectral method coherent with PN-97/H  on Spektrolab M5. The analysis results were presented in table 3.
4 84 M. Boldys, M. Stańczyk Steel type Results of the chemical composition analysis of the examined steel Content of chosen elements [%] C Mn Si P S Cr Cu C E Table 3 S235JRH 0,07 0,39 0,02 0,011 0,007-0,09 0,14 S355J2H 0,18 1,33 0,21 0,013 0,009-0,12 0,40 L360MB 0,05 0,58 0,26 0,012 0,006 0,03 0,08 0,16 C E coal equivalent The chemical composition analysis shown its compatibility with the values presented in norms Mechanical proprieties The mechanical proprieties of the examined steel were stated coherently with the norms PN- EN  and PN-EN  on the strength machine Wolpert Zwick 600 kn. The average examination results were presented in the table 4. On their basis it was stated that the mechanical proprieties have higher values than those given in PN-EN The examination results of tensile strength and the ductility limit for each steel and single samples are presented at fig Table 4 Mechanical proprieties of bands of S355J, S235JR and L360MB steel Steel types size [mm] R 0,2 [MPa] R m [MPa] A [%] according to PN min min. 26 S235JRH 6,3 measured scope average value according to PN min min. 22 S355J2H 4 measured scope average value according to PN R t0, min. 460 min. 20 L360MB 6,35 measured scope average value Fig. 2. Tensile strength and the ductility limit of a shape 100x150x6,3mm of S235JRH steel Rys. 2. Wytrzymałość na rozciąganie oraz granica plastyczności profilu 100x150x6,3mm ze stali S235JRH
5 The influence of the steel chemical 85 Fig. 3. Tensile strength and the ductility limit of a shape 100x100x4mm S355J2H steel Rys. 3. Wytrzymałość na rozciąganie oraz granica plastyczności profilu 100x100x4mm ze stali S355J2H Fig. 4. Tensile strength and the ductility limit of a shape φ273x6,35mm L360MB steel Rys. 4. Wytrzymałość na rozciąganie oraz granica plastyczności profilu φ273x6,35mm ze stali L360MB Fig. 5. R e /R m proportion for each steel Rys. 5. Stosunek R e /R m dla poszczególnych stali
6 86 M. Boldys, M. Stańczyk From the examination it is seen that the samples of S355J2H steel (R mapprox = 608 MPa) containing at least 1,33% of manganese and small amount of silicon, phosphorus, sulphur and copper have the highest strength (table 4). Simultaneously the samples made of the steel are characterised by a large amount of unit elongation (A approx = 36%) which shows its usefulness in cold plastic processing. Samples made of L360 MB steel, containing a small amount of coal (0,05%) and additions as manganese, silicon, phosphorus and chromium (table 4) are characterised by high value of strength (R mapprox = 507 MPa) but the smallest values of unit elongation among examined steel (A approx = 28%). The samples of L360MB steel, as the only ones, included chromium (0,03%) and had the highest amount of silicon (0,26%) which influenced the steel ductility Hardness measurement The hardness measurement was made according to norm PN-EN ISO  by the Vickers method with the load 98 N (HV 10). The detailed results of these measurements were presented on figures Fig. 6. Hardness distribution HV 10 on the section of welding cold forming shape 100x150x6,3 mm of S235JRH steel in the welding zone Rys. 6. Rozkład twardości HV 10 na przekroju zgrzewanego profilu zimnogiętego 100x150x6,3 mm ze stali S235JRH w obszarze zgrzeiny Fig. 7. Hardness distribution HV 10 on the section of welding cold forming shape 100x100x4 mm of S355J2H steel in the welding zone Rys. 7. Rozkład twardości HV 10 na przekroju zgrzewanego profilu zimnogiętego 100x100x4 mm ze stali S355J2H w obszarze zgrzeiny Fig. 8. Hardness distribution HV 10 on the section of bending shape 100x150x6,3 mm of S235JRH steel Rys. 8. Rozkład twardości HV 10 w obszarze gięcia profilu 100x150x6,3 mm ze stali S235JRH Fig. 9. Hardness distribution HV 10 on the section of bending 100x100x4 mm of S355J2H steel Rys. 9. Rozkład twardości HV 10 w obszarze gięcia profilu 100x100x4 mm ze stali S355J2H The achieved measurements proved predictable growth of hardness in the zone of welding, HAZ and in the zone of bending. In case of steel S235JRH the hardness growth in the zone of welding and HAZ amounted about 10,5% (z 172 HV do 190 HV), however in the zone of bending about 9% (do 210 HV). The distribution of measured hardness for steel S235JRH were presented in Fig. 6 and 8.
7 The influence of the steel chemical 87 Fig. 10. Hardness distribution HV 10 on the section of welding cold forming shape ø273x6,35mm of L360MB in the welding zone Rys. 10. Rozkład twardości HV 10 na przekroju zgrzewanego profilu zimnogiętego ø273x6,35mm ze stali L360MB w obszarze zgrzeiny In the samples taken from the shapes made of steel S355J2H with the hardness 190HV in the welding and its HAZ the hardness amounted to 208 HV (growth about 9,6%) and in the welding zone to 222HV (hardness growth about 18,5%) (Fig. 7 and 9). The zone welding made in the perimeter of the pipe shape Ø273x6,35 mm of L360MB steel is characterised by the welding hardness HV and HAZ HV with the steel hardness 220 HV (Fig. 10). In the welding zone and HAZ the hardness growth about 7,5% Microstructure examination The microstructure examination in the welding joint, the welding zone and the rectilinear sector of the shape of S235JRH and S355J2H steel was made on metallographic grinds treated with 2% nitric acid in ethyl alcohol (M1Fe) Results of structural analysis S235JRH steel Fig. 11. Microstructure in the rectilinear section of welded shape Rys. 11. Mikrostruktura w odcinku prostoliniowym kształtownika zgrzewanego Fig. 12. Microstructure in bending section of welded shape (near surface) Rys. 12. Mikrostruktura w odcinku giętym kształtownika zgrzewanego (przy powierzchni)
8 M. Boldys, M. Stańczyk S235JRH steel 88 Fig. 14. Microstructure in HAZ Rys. 14. Mikrostruktura w SWC Fig. 15. Microstructure in the joint section Rys. 15. Mikrostruktura w obszarze połączenia Fig. 16. Microstructure in HAZ Rys. 16. Mikrostruktura w SWC S235JRH steel Fig. 13. Microstructure in the joint section Rys. 13. Mikrostruktura w obszarze połączenia The shapes made of S235JRH steel are characterized by fine-grinded ferritic-pearlite structure (Fig ). They are characterized by high quality of producing and are free of welding errors (Fig ). In the welding axis there is a ferritic-banit structure (Fig. 13 and 14).
9 The influence of the steel chemical 89 S355JRH steel Fig. 17. Microstructure in the rectilinear section of welded shape Rys. 17. Mikrostruktura w odcinku prostoliniowym kształtownika zgrzewanego Fig. 18. Microstructure in bending section of welded shape (near surface) Rys. 18. Mikrostruktura w odcinku giętym kształtownika zgrzewanego (przy powierzchni) S355JRH steel Fig. 19. Microstructure in the joint section Rys. 19. Mikrostruktura w obszarze połączenia Fig. 20. Microstructure in HAZ Rys. 20. Mikrostruktura w SWC
10 M. Boldys, M. Stańczyk S355JRH steel 90 Fig. 21. Microstructure in the joint section Rys. 21. Mikrostruktura w obszarze połączenia Fig. 22. Microstructure in HAZ Rys. 22. Mikrostruktura w SWC In case of S355J2H steel there is also ferritic-pearlite structure (Fig. 17 and 18). In the welding zone and HAZ (Fig ) there are no welding errors. In this zone there is a ferritic-banit structure. 3. CONCLUSIONS On the basis of realized results analysis of the chemical composition, strength proprieties, hardness disposal S235JRH, S355J2H, L360MB steel and microstructure analysis steel S235JRH and S355J2H it was stated that: S355J2H steel has the highest strength (Rm = MPa). Among the examined steel it has the highest content of coal (0,18%) and manganese (1,33%). Moreover the sample was exposed to thermal-plastic treatment. L360MB steel shapes have lower than S355J2H steel strength (Rm = MPa). In their chemical composition there was 0,05% of coal and 0,57 0,67% of manganese and 0,020,04% of copper. This steel was also exposed to thermal-plastic treatment. lowest strength proprieties have welding shapes of S235JRH steel (Rm = MPa). This steel was normalized, it contained 0,07% of coal and the lowest amount of manganese 0,39%. S235JRH and S355J2H steel are characterized by the highest values of unit elongation (respectively Aapprox = 39 i 36%) which contained the lowest amount of silicon (respectively 0,02 i 0,21%) and highest than in samples of L360MB steel amount of sulphur (respectively 0,007 i 0,009%) samples of L360MB steel hale the lowest value of unit elongation (Aapprox = 28%), containing chromium (0,03%) and the lowest amount of sulphur (0,006%). on the basis of the examination it was stated that low amount of coal, manganese and phosphorus and high amount of sulphur has the biggest influence on steel ductility. On the basis of these examinations it was stated that there is an influence of steel chemical composition onto the possibilities of using it in cold shaping. The increase of manganese and coal amount has not a positive influence on the steel ductility. Simultaneously, the increase of amount of these elements positively influences the strength growth of steel (table 4).
11 The influence of the steel chemical 91 Literature 1. Praca zbiorowa pod redakcją Z. Jaśkiewicza: Poradnik inŝyniera samochodowego elementy i materiały. WKŁ, Warszawa Pafumi M.: Advanced High Strength Steel Technology in the 2006 Honda Civic. Creating Special Appeal with Steel. Honda R&D Americas, Inc., Praca zbiorowa pod redakcją J. Łukowskiego: Sprawozdanie z badań wykonywanych w ramach projektu celowego 6 ZR C/ PN-EN :205 (U) Wyroby walcowane na gorąco ze stali konstrukcyjnych. Część 1: Ogólne warunki techniczne dostawy. 5. Adamiec P., Dziubiński J.: Regeneracja i wytwarzanie warstw wierzchnich elementów maszyn transportowych. Wydawnictwo Politechniki Śląskiej, Gliwice H. Woźnica: Podstawy materiałoznawstwa. Wydawnictwo Politechniki Śląskiej, Gliwice PN-EN :205 (U) Wyroby walcowane na gorąco ze stali konstrukcyjnych. Część 2: Warunki techniczne dostawy stali konstrukcyjnych niestopowych. 8. PN-97/H Analiza chemiczna surówki, Ŝeliwa i stali. Oznaczanie zawartości węgla, manganu, krzemu, fosforu, siarki, chromu, niklu, miedzi, molibdenu, wanadu, glinu i niobu w stalach węglowych i niskostopowych metodą spektrometrii emisyjnej. 9. PN-EN Ogólne techniczne warunki dostawy stali i wyrobów stalowych. 10. PN-EN Kształtowniki zamknięte ze szwem wykonane na zimno ze stali konstrukcyjnych niestopowych i drobnoziarnistych. Warunki techniczne dostawy. 11. PN-EN ISO Metale. Pomiar twardości sposobem Vickersa. Część 4: Tablice wartości twardości. 12. PN-EN :1999 Rury stalowe przewodowe dla mediów palnych. 13. Dobrzański L.A.: Materiały inŝynierskie i projektowanie materiałowe. Podstawy nauki o materiałach i metaloznawstwo. WNT, Warszawa The research was made within BW 489/RT2/2007 Praca badawcza wykonana w ramach BW 489/RT2/2007 Received ; accepted in revised form